Effects of geometry and properties of fibre and matrix on overall. composite parameters


 Andrea Montgomery
 1 years ago
 Views:
Transcription
1 Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, by the authors Licensee IJASR Under Creative Commons License 3.0 Research article ISSN ffects of geometry and properties of fibre and matrix on overall composite parameters Yi Xiao 1, RiSong Qin 2, Manchu Mahalingam 1 1 Research School of ngineering, Australian National University, Canberra, ACT 2601, Australia 2 Fujian Port and Waterway Survey and Research Institute, 283 Yangqiao Road, Fuzhou, China DOI: /ijaser Abstract: To determine the overall material properties, 1, 2 and G 12, of a composite lamina, a finite element (F) simulation approach is presented and its results are compared with those from mechanics of materials. To investigate the effect of fibre s geometry on the overall composite properties, three different fibre s geometries are considered, in conjunction with two matrix materials and four fibre materials. Strand 7, the commercial F analysis software, is employed to conduct F simulation. The F results of the overall material properties of the composite, for different matrix s and fibre s geometries, and material properties, are compared with those from mechanics of materials approach. Key words: Composite lamina. Finite element approach, fiber geometry, fiber matrix. 1. Introduction Composite materials are playing an ever increasing role in supplying materials to satisfy the need for more demanding applications. These materials can be tailored to specific loading conditions which make them ideal to today s climate. Composite materials are superior to conventional materials, such as metals, due to their high strength to weight and stiffness to weight ratios. In classical mechanics, at a macrolevel, the material properties are always assumed to be homogeneous on an average basis, whereas at microlevel, i.e. inside the representative volume element (R), the material properties are heterogeneous. That is, at a microlevel, the heterogeneous microstructure is known and physical laws are known. The task of micromechanics is to find homogeneous material properties at a macrolevel based on the information of microstructure. These properties are often called overall material properties or effective material properties, and the process is also known as homogenization. Recently, some investigations have been made to the composite array using methods such as the homogenization method (Qin and Yang 2008). Grassi et al (Grassi et al. 2002) numerically examined the effect of fibre volume fraction of the through thickness Young s modulus. They found that an increase of 2% fibre volume fraction of Zfibres will induce an increase in the through thickness Young s modulus by a factor of 2235%. Qin et al (Qin 2004a; Qin 2004b; Yang and Qin 2004; Qin 2005) presented several boundary element micromechanics models for predicting effective properties of materials with defects or inclusions. Antoniou et al (Antoniou et al. 2009) developed a F model to predict mechanical behavior of glass/epoxy tubes under static loading. Xu et al (Xu et al. 2008) conducted an experiment on the plate size in determining the effective modulus. Yang and Qin (Yang and Qin 2001; Yang and Qin 2003) used F method to predict effective elastoplastic properties of composites. To determine the ranges of effective properties using various micromechanics models, the oigt and Reuss Rule (Gasik 1998) presented a *Corresponding author ( 792 Received on June 17, 2014; Accepted on August 19, 2014; Published on August 29, 2014
2 method to find the upper and lower bounds respectively of the stiffness for a composite material with arbitrary fibrematrix geometry. Micromechanics models were also used to determine effective properties of piezoelectric materials with cracks (Yu and Qin 1996; Qin and Yu 1997; Qin et al. 1998), microvoids (Qin and Yu 1998), and of human dentine materials (Qin and Swain 2004; Wang and Qin 2007; Wang and Qin 2011). Several other researchers have used representative unit cell models to investigate the dependence of component properties on composite materials (Levy and Papazian 1990; Tvergaard 1990; Bao et al. 1991; Zahl and McMeeking 1991; Li et al. 1995; Feng et al. 2003). In this paper, we examine the effect of geometries and properties of fibres on composites through F unit cell model. In particular, the three types of properties, namely 1, the Young s modulus in the fibre direction; 2, the Young s modulus in the transverse fibre direction; and G 12 the inplane shear modulus, are examined. By varying the shapes and material properties on the basis of mechanical and physical consideration the effect on the overall material properties can be explored. Moreover, the effect of the length in fibre direction on 1 is investigated and the minimum length required for achieving an acceptable converging result of 1 is obtained. 2. Background formulations In this section, two basic approaches for determining effective properties of fibre composites are briefly described in order to establish notations and provide a common source for reference in later sections. Moreover, material properties used in this work are listed in Section Mechanics of materials approach (MMA) The mechanics of materials method provides an accurate technique to calculate effective material properties of the fibre reinforced composites. These overall material properties can be used to predict the material behavior with various interfaces. The mechanics of materials approach determines the overall material properties due to their respective fibre and matrix volume fractions and constituent material properties. It assumes an average of stresses and strains to examine the global response. The first modulus to be determined is that of the composite material in the fibre direction (denoted as 1 axis), where, ε 1 applies to both the fibres and the matrix according to the basic assumption. 1 = f f + mm (1) q (1) is known as the rule of mixtures for the apparent Young s modulus of the composite material in the direction of the fibres. With the mechanics of materials method, the remain three properties can be determined using 2 m f = + m f f m, G12 GmG f = G + G m f f m ν12 = νmm + νf f (3) The rule appeared in q (2) is known as inverse rule of mixtures. 2.2 Finite element analysis (FA) (2) In order to obtain values for the material properties of fibre reinforced composites using a finite element method, the basic formulations are briefly described in this section. These differ to the mechanics of materials method in that they relate to the basic understanding of stress/strain relations and are not directly 793
3 related to the volume fractions as stated in Section ffective Young s modulus in fibre direction 1 and major Poisson ratio ν 12 1 and ν 12 can be determined by considering the loading case shown in Figure 1, where a stress σ 1 is applied in the fibre direction of the composite. The ffective Young s modulus and major Poisson ratio are, then, evaluated by σ σ d / σ d ε d / ε d ε = = =, ν 12 = = = ε1 1 ε1 / ε ε 1 ε1 / ε1 d d d d (4) Figure 1: Composite loaded in fibre direction If the left end is fixed and be defined as L represents the average displacement at the right end, the average strain can ε = L / L (5) Therefore, the major task for F calculation is to determine L and the average stress σ 1. This has been implemented into our F program ffective Transverse Young s modulus 2 Considering the loading case shown in Figure 2, the ffective Transverse Young s modulus 2 is defined as σ d / σ2 2 = = = ε2 ε d / σ d 2 2 ε d 2 2 where ε 2 = W / W. the major task for F calculation is to determine W and the average stress σ 2. (6) 794
4 Figure 2: Composite loaded in transverse direction ffective shear modulus G 12 The inplane shear modulus of a fibre reinforced composite can be determined by considering the loading case shown in Figure 3, a shear stress is applied over the boundary of the composite. G 12 τd / τ = = = γ γd / τd γd (7) Figure 3: Composite loaded with shear stress Considering the shear strain can be defined as u/y, where u is displacement in fibre direction and y stands for the vertical coordinate originated at the bottom of the composite, the task of F calculation, in this case, is to evaluate shear stress and the displacement u. From these equations, we can determine 1, 2 and G 12, noting that all other stress and strains are taken as zero except for the stress and strain along the direction for the material property being determined. 2.3 Material properties A list of common composite fibre and matrix materials were selected to model the geometries above. Fibres: 1) Carbon Fibre; 2) Kevlar; and 3) glass, and 4) Sglass) Matrix: 1) poxy Resin; and 2) Polyester Resin Tables 1 and 2 listed the mechanical properties of materials used in FA: 795
5 Table 1: Fibre Properties Fibre Material Carbon Fibre Kevlar 49 glass Sglass Young s Modulus 294GPa 131GPa 78GPa 89GPa Poisson s ratio Table 2: Matrix Properties Matrix Material (Resins) poxy Polyester Young s Modulus (tensile) 2.415GPa 2.467GPa Poisson s ratio Results and discussion To study effects of properties of each component and fibre s geometry on the overall properties of the composite, following 8 cases are considered: 1) carbon fibre with poxy Resin; 2) carbon fibre with Polyester Resin; 3) Kevlar49 with poxy Resin; 4) Kevlar49 with Polyester Resin; 5) glass with poxy Resin; 6) glass with Polyester Resin; 7) Sglass with poxy Resin; and 8) Sglass with Polyester Resin. For each case mentioned above, 6 combinations of geometry are involved: a) Rectangular matrix with circular fibres (RMCF); b) Rectangular matrix with hexagonal fibres (RMHF); c) Rectangular matrix with triangular fibres (RMTF); d) Square matrix with circular fibres (SMCF); e) Square matrix with hexagonal fibres (SMHF); and f) Square Matrix with triangular fibres (SMTF). The corresponding fibre volume fraction for each of these is: RMCF= ; RMHF= ; RMTF= ; SMCF= ; SMHF= ; SMTF= Figure 4: Geometry configurations of matrix and fibre (b=2 for RM and b=3 for SM) Figure 4 shows the geometry configuration of the unit cell used. It is obvious from Figure 1 that: a) total area is 6 for RM and 9 for SM; and the fibre s area is πr 2 = for circular fibre, 3 3/2 t 2 /2=3 3/ /2= for hexagonal fibre, and 0.5 for triangular fibre. The fibre volume fraction listed above is obtained based on these data. The finite element meshes used in the calculation are shown in Figure
6 a) SMCF b) SMHF c) SMTF Figure 5: Finite element meshes for square matrix with different fibre geometries The F results obtained are listed in Tables 310 and also shown in Figures 68. A comparison of the results between FA and MMA for 1 yield quite similar results. The average error between these results is within 3%, for all results, in determination of the 1. It indicates that MMA can provide acceptable accurate results for 1. Figure 6 shows a comparison between the results of varying fibre and matrix geometries. Figures 7 and 8 list the comparison in results between 2 and G 12, respectively, derived through MMA and FA. The difference of these results is within 8%, between all the results collected for 2 and G 12. As revealed by the graph the difference in results is not always constant. The square matrix with circular fibres, for example, has a smaller difference than the other models between MMA and FA results. This highlights the nonlinear nature of FA modelling software. Another point to note is that the values obtained for 1 using FA are lower than those from MMA, while the values obtained for 2 and G 12 using FA are higher than those from MMA. This is a result of the model thickness or the length in the fibre direction and will be discussed later in this paper. Table 3: Composites properties for carbon fibre with poxy Resin Properties 1 (GPa) 2 (GPa) G 12 (GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF Table 4: Composites properties for carbon fibre with Polyester Resin Properties 1 (GPa) 2 (GPa) G 12 (GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF
7 Properties Table 5: Composites properties for Kevlar49 with poxy Resin 1 (GPa) 2 (GPa) G 12 (GPa) 1(GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF Table 6: Composites properties for Kevlar49 with Polyester Resin Properties 1 (GPa) 2 (GPa) G 12 (GPa) 1(GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF Properties Table 7: Composites properties for glass with poxy Resin 1 (GPa) 2 (GPa) 1(GPa) G 12 (GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF
8 Properties Table 8: Composites properties for glass with Polyester Resin 1 (GPa) 2 (GPa) G 12 (GPa) 1(GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF Properties Table 9: Composites properties for Sglass with poxy Resin 1 (GPa) 2 (GPa) 1(GPa) G 12 (GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF Properties Table 10: Composites properties for Sglass with Polyester Resin 1 (GPa) 2 (GPa) G 12 (GPa) 1(GPa) Approach MMA FA MMA FA MMA FA RMCF RMHF RMTF SMCF SMHF SMTF
9 Figure 6: Comparison of 1 results from FA with those from MMA for the case of Carbon Fibre/poxy Resin Figure 7: Comparison of 2 results from FA with those from MMA for the case of Carbon Fibre/poxy Resin Figure 8: Comparison of 2 results from FA with those from MMA for the case of Carbon Fibre/poxy Resin 800
10 To study the effect of fibre and matrix materials on the overall material properties, several common matrix and fibre materials were selected for analysis and compared to investigate the effect material properties on the overall composite. It can be seen from Tables 310 that the material properties merely translate the corresponding values of 1, 2, and G 12 depending on the material property of components used. For example, polyester resin/matrix has a higher Young s modulus than epoxy resin, so the effect of matrix properties, compared to epoxy, is that it will increase the overall material properties 1 of the composite in a linear manner. Table 11: ariation of 1 due to variation of thickness in the 1 axis (fibre direction) 1axis thickness (mm) Stress(1axis) Displacement (1axis) Strain (GPa) Table 11 lists the 1 values obtained with respect to different thickness values of the model. That is, the thickness of the material in the fibre direction. It can be used to examine the effect of thickness on 1 when using FA. For the F results to converge towards the results obtained through MMA, a large thickness is needed to minimize end effects in the model. As the strain is a function of displacement over the original length, the strain values converge, that is, they become more uniform as the thickness increases. Nonetheless the thickness value also increases towards convergence, having the net effect of increasing the value of the 1. It could be thought that the displacement would decrease in a linear manner to the increase in thickness so that the expression L/L is held constant, this is however not the case. From this discussion it can be concluded that the ratio between thickness (fibre direction length) and the transverse direction length of the model needs to be at least 5:1 to minimize end effects in determination of the 1. For the 2 the converse ratio applies. The greater the ratio is, the more accurate the results obtained through FA are. 4. Conclusions From the analysis conducted, it can be seen that FA provides a sufficient means to calculate the overall material properties of the composite material and achieves results with acceptable accuracy. In the case of varying fibre geometries, triangular fibres exist in practice but are not common. Hexagonal fibres, not to be confused with a hexagonal array, are even less common. Nonetheless, FA also provides a method in which manufacturing of the constituent lamina of a composite is not necessary in order to begin initial testing and can therefore predict geometries that even do not exist in practice. Laboratory testing is still required before the final manufacture of composite materials, due to the inclusion of voids and matrix fibre interface. While FA provides a powerful tool to obtain premanufacturing analysis in order to determine if the manufacture of composites for specific applications is worthwhile in practice. The error rates, between the results obtained using MMA and FA is within 5% on average, which is an acceptable value. This is due to the fact that the 2 values had an approximate variance of 8% from the MMA values, whereas 1 and G 12 only had a variance of less than 3%. This error could be attributable to the fact that a composite 801
11 thickness of 10mm was used in contrast to the length of the model being 60mm. As discussed earlier in the results, the thickness has a direct effect on the overall material properties until convergence occurs. The ratio of thickness to length (see Table 11) needs to be considered to reduce end effects, and thus produce more accurate results. For convergence to occur with the 2, quite possibly a lesser thickness of 12mm could have been taken, or a greater length of material taken, or a combination of both to reduce the ratio of thickness to length, whereas with 1 the converse applies. It was found that the hexagonal fibres yielded the greatest results in overall material properties of the composite lamina. It is also noted that the hexagonal fibres had the highest fibre volume fraction of the varying geometries. It can therefore be stated from the results of this paper that the overall material properties are mainly dependant on the fibre and matrix volume fractions and are not dependant on geometry. Geometry will only define how the internal stresses and strains are dispersed within the material but, as the average strain was determined, this has no net effect on the overall material properties. In practice, however, the internal stresses due to varying the fibrematrix geometries will have an impact on the fibrematrix interface and will invariably affect the overall material properties and should not be overlooked. 5. References 1. Antoniou, A.., Kensche, C. and Philippidis, T. P., Mechanical behavior of glass/epoxy tubes under combined static loading. Part II: alidation of FA progressive damage model. Composites Science and Technology, 69(13), pp Bao, G., Hutchinson, J. W. and McMeeking, R. M., Particle reinforcement of ductile matrices against plasticflow and creep. Acta Metallurgica t Materialia, 39(8), pp Feng, X. Q., Mai, Y. W. and Qin, Q. H., A micromechanical model for interpenetrating multiphase composites. Computational Materials Science, 28(3), pp Gasik, M. M., Micromechanical modelling of functionally graded materials. Computational Materials Science, 13(13), pp Grassi, M., Zhang, X. and Meo, M., Prediction of stiffness and stresses in zfibre reinforced composite laminates. Composites Part aapplied Science and Manufacturing, 33(12), pp Levy, A. and Papazian, J. M., Tensile properties of short fiberreinforced sic/al composites.2. Finiteelement analysis. Metallurgical Transactions aphysical Metallurgy and Materials Science, 21(2), pp Li, Z. H., Schmauder, S., Wanner, A. and Dong, M., xpressions to characterize the flow behavior of particlereinforced composites based on axisymmetrical unitcell models. Scripta Metallurgica t Materialia, 33(8), pp Qin, Q. H., 2004a. Material properties of piezoelectric composites by BM and homogenization method. Composite structures, 66(1), pp Qin, Q. H., 2004b. MicromechanicsB solution for properties of piezoelectric materials with defects. ngineering analysis with boundary elements, 28(7), pp Qin, Q. H., MicromechanicsBM Analysis for Piezoelectric Composites. Tsinghua Science & Technology, 10(1), pp
12 11. Qin, Q. H., Mai, Y. W. and Yu, S. W., ffective moduli for thermopiezoelectric materials with microcracks. International Journal of Fracture, 91(4), pp Qin, Q. H. and Swain, M.., A micromechanics model of dentin mechanical properties. Biomaterials, 25(20), pp Qin, Q. H. and Yang, Q. S. (2008). MacroMicro Theory on Multifield Coupling Behaivor of Hetereogenous Materials. Beijing, Higher ducation Press and Springer. 14. Qin, Q. H. and Yu, S. W. (1997). Using MoriTanaka method for effective moduli of cracked thermopiezoelectric materials. ICF 9Sydney, Australia Qin, Q. H. and Yu, S. W., ffective moduli of piezoelectric material with microcavities. International Journal of Solids and Structures, 35(36), pp Tvergaard,., Analysis of tensile properties for a whiskerreinforced metal matrix composite. Acta Metallurgica t Materialia, 38(2), pp Wang, Y. and Qin, Q. H., A generalized self consistent model for effective elastic moduli of human dentine. Composites science and technology, 67(7), pp Wang, Y. and Qin, Q. H., Micromechanics for determining effective material properties of dentine composites. Advances in ngineering Mechanics, 1, pp Xu, L. M., Li, C., Fan, H. and Wang, B., lastic property prediction by finite element analysis with random distribution of materials for tungsten/silver composite. Journal of Materials Science, 43(17), pp Yang, Q. S. and Qin, Q. H., Fiber interactions and effective elastoplastic properties of shortfiber composites. Composite structures, 54(4), pp Yang, Q. S. and Qin, Q. H., Modelling the effective elastoplastic properties of unidirectional composites reinforced by fibre bundles under transverse tension and shear loading. Materials Science and ngineering: A, 344(1), pp Yang, Q. S. and Qin, Q. H., Micromechanical analysis of composite materials by BM. ngineering Analysis with Boundary lements, 28(8), pp Yu, S. W. and Qin, Q. H., Damage analysis of thermopiezoelectric properties: Part II. ffective crack model. Theoretical and Applied Fracture Mechanics, 25(3), pp Zahl, D. B. and McMeeking, R. M., The influence of residualstress on the yielding of metal matrix composites. Acta Metallurgica t Materialia, 39(6), pp
Prediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationMODELLING OF THE THERMOMECHANICAL PROPERTIES OF WOVEN COMPOSITES DURING THE CURE
TH 9 TH INTRNATIONAL ONFRN ON OMPOSIT MATRIALS MODLLING OF TH THRMOMHANIAL PROPRTIS OF WOVN OMPOSITS DURING TH UR L. Khoun,, K.S. hallagulla,, P. Hubert Department of Mechanical ngineering, McGill University,
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationStressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationNUMERICAL MODELING ON ELECTRIC RESPONSE OF FIBRE ORIENTATION OF COMPOSITES WITH PIEZOELECTRICITY
www.arpapress.com/volumes/vol15issue2/ijrras_15_2_08.pdf NUMRICAL MODLIN ON LCTRIC RSPONS OF FIBR ORINTATION OF COMPOSITS WITH PIZOLCTRICITY CheukYu Lee, Qing H. Qin and uy Walpole Research School of
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationTHE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF ORIENTED STRANDBOARD: A FINITE ELEMENT SIMULATION
Proceedings of McMat5: 5 Joint ASME/ASCE/SES Conference on Mechanics and Materials June 13, 5, Baton Rouge, Louisiana, USA 255 THE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationNanoindentation of Fibrous Composite Microstructures: Experimentation and Finite Element Investigation. Mark Hardiman
Nanoindentation of Fibrous Composite Microstructures: Experimentation and Finite Element Investigation Mark Hardiman Materials and Surface Science Institute (MSSI), Department of Mechanical and Aeronautical
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationDepartment of Mechanical Engineering, National Institute of Technology Rourkela, Rourkela , India
Composites, Article ID 629175, 12 pages http://dx.doi.org/10.1155/2014/629175 Research Article Effect of Fiber Geometry and Representative Volume Element on Elastic and Thermal Properties of Unidirectional
More informationEvaluation Axisymmetric Analysis of Thermal Stress Residual Near Fiber/Epoxy Interface
Materials Research, Vol. 12, No. 2, 133137, 2009 2009 Evaluation Axisymmetric Analysis of Thermal Stress Residual Near Fiber/Epoxy Interface Aboubakar Seddik Bouchikhi Department of Mechanical Engineering,
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationEffect of fibre shape on transverse thermal conductivity of unidirectional composites
Sādhanā Vol. 4, Part 2, April 25, pp. 53 53. c Indian Academy of Sciences Effect of fibre shape on transverse thermal conductivity of unidirectional composites B RAGHAVA RAO,, V RAMACHANDRA RAJU 2 and
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationAN EFFECTIVE SOLUTION OF THE COMPOSITE (FGM S) BEAM STRUCTURES
Engineering MECHANICS, Vol. 15, 2008, No. 2, p. 115 132 115 AN EFFECTIVE SOLUTION OF THE COMPOSITE (FGM S) BEAM STRUCTURES Justín Murín, Vladimír Kutiš* The additive mixture rules have been extended for
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationAn ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials
An ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials by Shari Lynn King A thesis presented to the University of Waterloo in fulfillment of the thesis requirement for
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationAuthors: Correspondence: ABSTRACT:
MultiScale Modeling of the Impact and Failure of Fiber Reinforced Polymer Structures using DIGIMAT to LSDYNA Interface Authors: L. Adam, R. Assaker & R. Ramaya exstream engineering S.A. 7, Rue du Bosquet.
More informationLaminated Composite Plates and Shells
Jianqiao Ye Laminated Composite Plates and Shells 3D Modelling With 62 Figures Springer Table of Contents 1. Introduction to Composite Materials 1 1.1 Introduction 1 1.2 Classification of Composite Materials
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationIn Situ Ultrasonic NDT of Fracture and Fatigue in Composites
ECNDT 26  Mo.2.6.5 In Situ Ultrasonic NDT of Fracture and Fatigue in Composites I. SOLODOV, K. PFLEIDERER, and G. BUSSE Institute for Polymer Testing and Polymer Science (IKP), Nondestructive Testing
More information2 Experiment of GFRP bolt
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FATIGUE LIFE EVALUATION OF BOLT MADE OF WOVEN FABRIC FRP Takeshi INOUE*, Hiroaki NAKAI**, Tetsusei KURASHIKI**, Masaru ZAKO**, Yuji KOMETANI*** *Graduate
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationSize Effect of Clay Filler Particles on Mechanical Properties of Pultruded Polymer Composites Under Shear Loading
Minnesota State University, Mankato Cornerstone: A Collection of Scholarly and Creative Works for Minnesota State University, Mankato All Theses, Dissertations, and Other Capstone Projects Theses, Dissertations,
More informationSchool of Materials Science and Engineering, UNSW Sydney, Australia 2. School of Mechanical and Manufacturing Engineering, UNSW Sydney, Australia
2 st International Conference on Composite Materials Xi an, 2025 th August 207 PREDICTING THE EFFECT OF TEMPERATURE ON MATRIX CRACKING IN THERMOSET COMPOSITES USING A STRAIN INVARIANT APPROACH Akhila
More informationON HOMOGENIZATION AND DEHOMOGENIZATION OF COMPOSITE MATERIALS. A Thesis. Submitted to the Faculty. Drexel University.
ON HOMOGENIZATION AND DEHOMOGENIZATION OF COMPOSITE MATERIALS A Thesis Submitted to the Faculty of Drexel University by Chang (Karen) Yan in partial fulfillment of the requirements for the degree of Doctor
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More informationMODELING AND ANALYSIS OF HEXAGONAL UNIT CELL FOR THE PREDICTION OF EFFECTIVE THERMAL CONDUCTIVITY
International Journal of Mechanical Engineering and Technology (IJMET) Volume 8, Issue 5, May 2017, pp. 651 655, Article ID: IJMET_08_05_071 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=8&itype=5
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationThe Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar
The Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar DUMITRU BOLCU 1 *, MIHAELA SAVA 2, ALIN DINITA 3, COSMIN
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationA coupled field finite element model to predict actuation properties of piezoelectrically actuated bistable composites.
A coupled field finite element model to predict actuation properties of piezoelectrically actuated bistable composites. P.F.Giddings, C.R.Bowen, H.A.Kim University of Bath, UK Dept. Mech. ng, University
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationFinite Element Modeling of Residual Thermal Stresses in FiberReinforced Composites Using Different Representative Volume Elements
Proceedings o the World Congress on Engineering 21 Vol II WCE 21, June 3  July 2, 21, London, U.K. Finite Element Modeling o Residual Thermal Stresses in FiberReinorced Composites Using Dierent Representative
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationMicromechanics Analysis of Fiber Reinforced Composite
Micromechanics Analysis of Fiber Reinforced Composite Paresh K Katariya Student, MECAD/CAM, Department of mechanical engineering, Shree S ad Vidya Mandal Institute of Technology, Bharuch, Gujarat, India
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationSoufiane Belhouideg. Keywords Composite materials, homogenization method, Eshelby s inclusion problem.
Prediction of effective mechanical properties of composite materials using homogenization approach: Application to tungsten fiber reinforced bulk metallic glass matrix composite Soufiane Belhouideg Abstract
More informationPredicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics
Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics Neelam Mishra 1, and Kaushik Das *1 1 School of Minerals Metallurgical and Materials Engineering, Indian
More informationCombined IsotropicKinematic Hardening Laws with Anisotropic Backstress Evolution for Orthotropic FiberReinforced Composites
Combined IsotropicKinematic Hardening Laws with Antropic Backstress Evolution for Orthotropic Fiber Reinforced Composites Combined IsotropicKinematic Hardening Laws with Antropic Backstress Evolution
More informationThermoMechanical Response of Functionally Graded Materials for Extreme Environments
ThermoMechanical Response of Functionally Graded Materials for Extreme Environments Introduction In recent years, functionally graded materials (FGMs) have attracted much interest in a wide range of engineering
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationDEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY COMPOSITES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 2014 DEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY
More informationDiscrete Element Modelling of a Reinforced Concrete Structure
Discrete Element Modelling of a Reinforced Concrete Structure S. Hentz, L. Daudeville, F.V. Donzé Laboratoire Sols, Solides, Structures, Domaine Universitaire, BP 38041 Grenoble Cedex 9 France sebastian.hentz@inpg.fr
More informationThe overall elastic moduli of orthotropic composite and description of orthotropic damage of materials
International Journal of Solids and Structures 37 (2000) 6755±6771 www.elsevier.com/locate/ijsolstr The overall elastic moduli of orthotropic composite and description of orthotropic damage of materials
More informationModelling of multiaxial ultimate elastic wall stress (UEWS) test for glass fibre reinforced epoxy (GRE) composite pipes
pplied Mechanics and Materials Vol. 367 (013) pp 113117 Online available since 013/ug/16 at www.scientific.net (013) Trans Tech Publications, Switzerland doi:10.408/www.scientific.net/mm.367.113 Modelling
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationHOMOGENIZATION AND UNCERTAINTY ANALYSIS FOR FIBER REINFORCED COMPOSITES
HOMOGENIZATION AND UNCERTAINTY ANALYSIS FOR FIBER REINFORCED COMPOSITES By JINUK KIM A DISSERTATION PRESENTED TO THE GRADUATE SCHOOL OF THE UNIVERSITY OF FLORIDA IN PARTIAL FULFILLMENT OF THE REQUIREMENTS
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationDesign and optimization of a variable stiffness composite laminate
th World Congress on Structural and Multidisciplinary Optimisation 07 th  th, June 05, Sydney Australia Design and optimization of a variable stiffness composite laminate Yan Zhang, Fenfen Xiong Qian
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationMechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
IJRMET Vo l. 4, Is s u e Sp l  1, No v 2013 Ap r i l 2014 ISSN : 22495762 (Online ISSN : 22495770 (Print Mechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMultiscale analyses of the behaviour and damage of composite materials
Multiscale analyses of the behaviour and damage of composite materials Presented by Didier BAPTISTE ENSAM, LIM, UMR CNRS 8006 151 boulevard de l hôpital l 75013 PARIS, France Research works from: K.Derrien,
More informationMODELLING INTERACTION EFFECT OF NANOSILICA PARTICLES ON NANOSILICA/EPOXY COMPOSITE STIFFNESS
MODELLING INTERACTION EFFECT OF NANOSILICA PARTICLES ON NANOSILICA/EPOXY COMPOSITE STIFFNESS Mulyadi a*, I. Gitman a, C. Pinna a, C. Soutis b a Department of Mechanical Engineering, The University of Sheffield,
More informationFatigue Damage Development in a Steel Based MMC
Fatigue Damage Development in a Steel Based MMC V. Tvergaard 1,T.O/ rts Pedersen 1 Abstract: The development of fatigue damage in a toolsteel metal matrix discontinuously reinforced with TiC particulates
More informationTENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES
TENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES C. Qian 1 *, R. P. L. Nijssen 1, D. D. Samborsky 2, C.Kassapoglou 3, Z. Gürdal 3, G. Q. Zhang 4 1 Knowledge Centre Wind turbine Materials and
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More information